LMucko/crystallography-open-database huggingface dataset:
Average model of incommensurate crystal structure (Ca7Sr7)(Cu23.62Bi0.38)O41
Arakcheeva, A.V.; Shamrai, V.F.; Kristallografiya 38 (1993) 40–51; doi:

data_1534621
_publ_section_title
;
 Average model of incommensurate crystal structure
 (Ca7Sr7)(Cu23.62Bi0.38)O41
;
_journal_name_full               Kristallografiya
_journal_page_first              40
_journal_page_last               51
_journal_volume                  38
_journal_year                    1993
_chemical_formula_sum            'Bi0.38 Ca8.2 Cu23.62 O41 Sr5.8'
_chemical_name_systematic        'Ca8.2 Sr5.8 Cu23.62 Bi0.38 O41'
_space_group_IT_number           37
_symmetry_space_group_name_Hall  'C 2 -2c'
_symmetry_space_group_name_H-M   'C c c 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.942
_cell_length_b                   11.387
_cell_length_c                   27.46
_cell_volume                     4046.795
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Arakcheeva_KRISAJ_1993_1340.cif
_cod_data_source_block           Bi0.38Ca8.2Cu23.62O41Sr5.8
_cod_database_code               1534621
Transition metal-gallium ordering in Hf Co Ga2 and Hf Ni Ga2
Schlueter, M.; Heying, B.; Poettgen, R.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (42,1987-) 58 (2003) 16–21; doi:

data_7222491
_publ_section_title
;
 Transition metal-gallium ordering in Hf Co Ga2 and Hf Ni Ga2
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (42,1987-)
;
_journal_page_first              16
_journal_page_last               21
_journal_volume                  58
_journal_year                    2003
_chemical_formula_sum            'Ga2 Hf Ni'
_chemical_name_systematic        'Hf Ni Ga2'
_space_group_IT_number           107
_symmetry_space_group_name_Hall  'I 4 -2'
_symmetry_space_group_name_H-M   'I 4 m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            20
_cell_length_a                   12.24
_cell_length_b                   12.24
_cell_length_c                   8.093
_cell_volume                     1212.474
_citation_journal_id_ASTM        ZNBSEN
_cod_data_source_file            Schlueter_ZNBSEN_2003_807.cif
_cod_data_source_block           Ga2Hf1Ni1
_cod_original_formula_sum        'Ga2 Hf1 Ni1'
_cod_database_code               7222491
Nitridsulfidhalogenide der leichten Lanthanide vom Typ M6 N3 S4 X (M = La - Nd; X = Cl, Br) mit ausgeordneten Sulfid- und Halogenid-Lagen
Lissner, F.; Schleid, T.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (42,1987-) 57 (2002) 1079–1084; doi:

data_7222492
_publ_section_title
;
 Nitridsulfidhalogenide der leichten Lanthanide vom Typ M6 N3 S4 X (M = La
 - Nd; X = Cl, Br) mit ausgeordneten Sulfid- und Halogenid-Lagen
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (42,1987-)
;
_journal_page_first              1079
_journal_page_last               1084
_journal_volume                  57
_journal_year                    2002
_chemical_formula_sum            'Br Ce6 N3 S4'
_chemical_name_systematic        'Ce6 N3 S4 Br'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.5231
_cell_length_b                   4.0752
_cell_length_c                   27.474
_cell_volume                     1290.150
_citation_journal_id_ASTM        ZNBSEN
_cod_data_source_file            Lissner_ZNBSEN_2002_752.cif
_cod_data_source_block           Br1Ce6N3S4
_cod_original_cell_volume        1290.15
_cod_original_formula_sum        'Br1 Ce6 N3 S4'
_cod_database_code               7222492
Bis(trifluormethyl)trioxid: a first structure of a straightchain trioxide
Gobbato, K.I.; Oberhammer, H.; Klapdor, M.F.; Poll, W.; Willner, H.; Mootz, D.; Angewandte Chemie (Edition international) 34 (1995) 2244–2245; doi:

data_1534622
_publ_section_title
;
 Bis(trifluormethyl)trioxid: a first structure of a straightchain trioxide
;
_journal_name_full               'Angewandte Chemie (Edition international)'
_journal_page_first              2244
_journal_page_last               2245
_journal_volume                  34
_journal_year                    1995
_chemical_formula_sum            'C2 F6 O3'
_chemical_name_systematic        '(C F3)2 O3'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                78.91
_cell_angle_beta                 86.12
_cell_angle_gamma                83.49
_cell_formula_units_Z            2
_cell_length_a                   4.81
_cell_length_b                   7.477
_cell_length_c                   7.993
_cell_volume                     279.966
_citation_journal_id_ASTM        ACIEAY
_cod_data_source_file            Gobbato_ACIEAY_1995_1780.cif
_cod_data_source_block           C2F6O3
_cod_original_cell_volume        279.9661
_cod_database_code               1534622
Crystal structure of a phase of disomatic type of a variable composition CaAl(Al, V, M(I))2 (V, M(II)) (Si, Al)2O10, where M(I)=Mg, M(II)=Al,Fe.Mn.Ti, Mg; and its polytype modifications and structural homologues
Arakcheeva, A.V.; Ivanov, I.T.; Kristallografiya 38 (1993) 144–161; doi:

data_1534623
_publ_section_title
;
 Crystal structure of a phase of disomatic type of a variable composition
 CaAl(Al, V, M(I))2 (V, M(II)) (Si, Al)2O10, where M(I)=Mg,
 M(II)=Al,Fe.Mn.Ti, Mg; and its polytype modifications and structural
 homologues
;
_journal_name_full               Kristallografiya
_journal_page_first              144
_journal_page_last               161
_journal_volume                  38
_journal_year                    1993
_chemical_formula_sum
'Al15.14 Ca4 Fe0.026 Mg Mn0.024 O40 Si2.36 Ti0.3 V5.15'
_chemical_name_systematic
;
Ca4 Al15.14 V5.15 Mg Fe0.026 Ti0.3 Mn0.024 Si2.36 O40
;
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                106.24
_cell_angle_beta                 95.71
_cell_angle_gamma                124.47
_cell_formula_units_Z            1
_cell_length_a                   10.273
_cell_length_b                   10.634
_cell_length_c                   8.808
_cell_volume                     720.098
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Arakcheeva_KRISAJ_1993_1369.cif
_cod_data_source_block           Al15.14Ca4Fe0.026Mg1Mn0.024O40Si2.36Ti0.3V5.15
_cod_original_cell_volume        720.0975
_cod_original_formula_sum
'Al15.14 Ca4 Fe0.026 Mg1 Mn0.024 O40 Si2.36 Ti0.3 V5.15'
_cod_database_code               1534623
High-temperature synthesis, single-crystal X-ray structure determination and solid-state NMR investigations of Ba7 (Si O4) (B O3)3 C N and Sr7 (Si O4) (B O3)3 C N
Schmid, S.; Senker, J.; Schnick, W.; Journal of Solid State Chemistry 174 (2003) 221–228; doi:

data_1534624
_publ_section_title
;
 High-temperature synthesis, single-crystal X-ray structure determination
 and solid-state NMR investigations of Ba7 (Si O4) (B O3)3 C N and Sr7 (Si
 O4) (B O3)3 C N
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              221
_journal_page_last               228
_journal_volume                  174
_journal_year                    2003
_chemical_formula_sum            'C B3 Ba7 N O13 Si'
_chemical_name_systematic        'Ba7 (Si O4) (B O3)3 (C N)'
_space_group_IT_number           186
_symmetry_space_group_name_Hall  'P 6c -2c'
_symmetry_space_group_name_H-M   'P 63 m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   11.299
_cell_length_b                   11.299
_cell_length_c                   7.334
_cell_volume                     810.871
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Schmid_JSSCBI_2003_899.cif
_cod_data_source_block           C1B3Ba7N1O13Si1
_cod_original_cell_volume        810.8706
_cod_original_formula_sum        'C1 B3 Ba7 N1 O13 Si1'
_cod_database_code               1534624
Nitridsulfidhalogenide der leichten Lanthanide vom Typ M6 N3 S4 X (M = La - Nd; X = Cl, Br) mit ausgeordneten Sulfid- und Halogenid-Lagen
Lissner, F.; Schleid, T.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (42,1987-) 57 (2002) 1079–1084; doi:

data_7222493
_publ_section_title
;
 Nitridsulfidhalogenide der leichten Lanthanide vom Typ M6 N3 S4 X (M = La
 - Nd; X = Cl, Br) mit ausgeordneten Sulfid- und Halogenid-Lagen
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (42,1987-)
;
_journal_page_first              1079
_journal_page_last               1084
_journal_volume                  57
_journal_year                    2002
_chemical_formula_sum            'Br La6 N3 S4'
_chemical_name_systematic        'La6 N3 S4 Br'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.5923
_cell_length_b                   4.1085
_cell_length_c                   27.656
_cell_volume                     1317.171
_citation_journal_id_ASTM        ZNBSEN
_cod_data_source_file            Lissner_ZNBSEN_2002_753.cif
_cod_data_source_block           Br1La6N3S4
_cod_original_formula_sum        'Br1 La6 N3 S4'
_cod_database_code               7222493
Hexaamminechromium diamminetetrafluorochromate(III) bis(tetrafluoroborate)
Goebbels, D.; Meyer, G.; Private Communication 2001 (2001) 1–1; doi:

data_1534625
_publ_section_title
;
 Hexaamminechromium diamminetetrafluorochromate(III)
 bis(tetrafluoroborate)
;
_journal_name_full               'Private Communication'
_journal_page_first              1
_journal_page_last               1
_journal_volume                  2001
_journal_year                    2001
_chemical_formula_sum            'B2 Cr2 F12 H24 N8'
_chemical_name_systematic        '(Cr (N H3)6) (Cr (N H3)2 F4) (B F4)2'
_space_group_IT_number           127
_symmetry_space_group_name_Hall  '-P 4 2ab'
_symmetry_space_group_name_H-M   'P 4/m b m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   10.5322
_cell_length_b                   10.5322
_cell_length_c                   7.7371
_cell_volume                     858.255
_citation_journal_id_ASTM        PRICO6
_cod_data_source_file            Goebbels_PRICO6_2001_248.cif
_cod_data_source_block           H24B2Cr2F12N8
_cod_original_cell_volume        858.2551
_cod_original_formula_sum        'H24 B2 Cr2 F12 N8'
_cod_database_code               1534625
The ordering of Ca and Sr atoms in the structure of (Ca0.5 Sr0.5) (Cu0.75 Bi0.25) O2
Arakcheeva, A.V.; Shamrai, V.F.; Leonyuk, L.I.; Lubman, G.U.; Kristallografiya 39 (1994) 928–931; doi:

data_1534626
_publ_section_title
;
 The ordering of Ca and Sr atoms in the structure of (Ca0.5 Sr0.5) (Cu0.75
 Bi0.25) O2
;
_journal_name_full               Kristallografiya
_journal_page_first              928
_journal_page_last               931
_journal_volume                  39
_journal_year                    1994
_chemical_formula_sum            'Bi0.5 Ca Cu1.5 O4 Sr'
_chemical_name_systematic        '(Ca Sr) (Cu1.5 Bi0.5) O4'
_space_group_IT_number           123
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   5.465
_cell_length_b                   5.465
_cell_length_c                   3.2143
_cell_volume                     95.999
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Arakcheeva_KRISAJ_1994_1435.cif
_cod_data_source_block           Bi0.5Ca1Cu1.5O4Sr1
_cod_original_cell_volume        95.99901
_cod_original_formula_sum        'Bi0.5 Ca1 Cu1.5 O4 Sr1'
_cod_database_code               1534626
High-temperature synthesis, single-crystal X-ray structure determination and solid-state NMR investigations of Ba7 (Si O4) (B O3)3 C N and Sr7 (Si O4) (B O3)3 C N
Schmid, S.; Senker, J.; Schnick, W.; Journal of Solid State Chemistry 174 (2003) 221–228; doi:

data_1534627
_publ_section_title
;
 High-temperature synthesis, single-crystal X-ray structure determination
 and solid-state NMR investigations of Ba7 (Si O4) (B O3)3 C N and Sr7 (Si
 O4) (B O3)3 C N
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              221
_journal_page_last               228
_journal_volume                  174
_journal_year                    2003
_chemical_formula_sum            'C B3 N O13 Si Sr7'
_chemical_name_systematic        'Sr7 (Si O4) (B O3)3 (C N)'
_space_group_IT_number           186
_symmetry_space_group_name_Hall  'P 6c -2c'
_symmetry_space_group_name_H-M   'P 63 m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   10.813
_cell_length_b                   10.813
_cell_length_c                   6.952
_cell_volume                     703.935
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Schmid_JSSCBI_2003_900.cif
_cod_data_source_block           C1B3N1O13Si1Sr7
_cod_original_cell_volume        703.9354
_cod_original_formula_sum        'C1 B3 N1 O13 Si1 Sr7'
_cod_database_code               1534627
Nitridsulfidhalogenide der leichten Lanthanide vom Typ M6 N3 S4 X (M = La - Nd; X = Cl, Br) mit ausgeordneten Sulfid- und Halogenid-Lagen
Lissner, F.; Schleid, T.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (42,1987-) 57 (2002) 1079–1084; doi:

data_7222494
_publ_section_title
;
 Nitridsulfidhalogenide der leichten Lanthanide vom Typ M6 N3 S4 X (M = La
 - Nd; X = Cl, Br) mit ausgeordneten Sulfid- und Halogenid-Lagen
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (42,1987-)
;
_journal_page_first              1079
_journal_page_last               1084
_journal_volume                  57
_journal_year                    2002
_chemical_formula_sum            'Br N3 Nd6 S4'
_chemical_name_systematic        'Nd6 N3 S4 Br'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.3859
_cell_length_b                   4.0094
_cell_length_c                   27.113
_cell_volume                     1237.725
_citation_journal_id_ASTM        ZNBSEN
_cod_data_source_file            Lissner_ZNBSEN_2002_754.cif
_cod_data_source_block           Br1N3Nd6S4
_cod_original_formula_sum        'Br1 N3 Nd6 S4'
_cod_database_code               7222494
Aufbau und Abbau von (N H4) (B F4) und (H3 N)-(B F3)
Goebbels, D.; Meyer, G.; Zeitschrift fuer Anorganische und Allgemeine Chemie 628 (2002) 1799–1805; doi:

data_1534628
_publ_section_title
;
 Aufbau und Abbau von (N H4) (B F4) und (H3 N)-(B F3)
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              1799
_journal_page_last               1805
_journal_volume                  628
_journal_year                    2002
_chemical_formula_sum            'B F3 H3 N'
_chemical_name_systematic        '(H3 N) (B F3)'
_space_group_IT_number           61
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0726
_cell_length_b                   8.0048
_cell_length_c                   9.2431
_cell_volume                     597.285
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Goebbels_ZAACAB_2002_249.cif
_cod_data_source_block           H3B1F3N1
_cod_original_formula_sum        'H3 B1 F3 N1'
_cod_database_code               1534628
Crystal structure of baikovite mineral
Arakcheeva, A.V.; Kristallografiya 40 (1995) 245–252; doi:

data_1534629
_publ_section_title
;
 Crystal structure of baikovite mineral
;
_journal_name_full               Kristallografiya
_journal_page_first              245
_journal_page_last               252
_journal_volume                  40
_journal_year                    1995
_chemical_formula_sum            'Al2.16 Ca1.07 Mg1.397 O10 Si0.9 Ti1.48'
_chemical_name_systematic
;
Ca1.07 Mg0.625 Ti0.31 ((Al.55 Si.45)2 O6) (Al (Mg0.386 Ti.585 Al0.03)2 O4)
;
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                105.98
_cell_angle_beta                 96.05
_cell_angle_gamma                124.76
_cell_formula_units_Z            4
_cell_length_a                   10.425
_cell_length_b                   10.799
_cell_length_c                   8.924
_cell_volume                     748.424
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Arakcheeva_KRISAJ_1995_1484.cif
_cod_data_source_block           Al2.16Ca1.07Mg1.397O10Si0.9Ti1.48
_cod_original_cell_volume        748.4243
_cod_database_code               1534629
Nitridsulfidhalogenide der leichten Lanthanide vom Typ M6 N3 S4 X (M = La - Nd; X = Cl, Br) mit ausgeordneten Sulfid- und Halogenid-Lagen
Lissner, F.; Schleid, T.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (42,1987-) 57 (2002) 1079–1084; doi:

data_7222495
_publ_section_title
;
 Nitridsulfidhalogenide der leichten Lanthanide vom Typ M6 N3 S4 X (M = La
 - Nd; X = Cl, Br) mit ausgeordneten Sulfid- und Halogenid-Lagen
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (42,1987-)
;
_journal_page_first              1079
_journal_page_last               1084
_journal_volume                  57
_journal_year                    2002
_chemical_formula_sum            'Br N3 Pr6 S4'
_chemical_name_systematic        'Pr6 N3 S4 Br'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.4542
_cell_length_b                   4.0421
_cell_length_c                   27.293
_cell_volume                     1263.639
_citation_journal_id_ASTM        ZNBSEN
_cod_data_source_file            Lissner_ZNBSEN_2002_755.cif
_cod_data_source_block           Br1N3Pr6S4
_cod_original_formula_sum        'Br1 N3 Pr6 S4'
_cod_database_code               7222495
Al and Tb ordering in the multiplied by nine cell of the Y0.8 (Tb3+)0.129 Ba2 (Cu2.725 (Tb4+)0.053) Al0.11 O6.4
Arakcheeva, A.V.; Lubman, G.U.; Leonyuk, L.I.; Shamrai, V.F.; Kristallografiya 40 (1995) 833–841; doi:

data_1534631
_publ_section_title
;
 Al and Tb ordering in the multiplied by nine cell of the Y0.8 (Tb3+)0.129
 Ba2 (Cu2.725 (Tb4+)0.053) Al0.11 O6.4
;
_journal_name_full               Kristallografiya
_journal_page_first              833
_journal_page_last               841
_journal_volume                  40
_journal_year                    1995
_chemical_formula_sum            'Al0.11 Ba2 Cu2.725 O6.4 Tb0.182 Y0.8'
_chemical_name_systematic
'Y0.8 Tb0.129 Ba2 (Cu2.725 Tb0.053) Al0.11 O6.4'
_space_group_IT_number           123
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            9
_cell_length_a                   11.606
_cell_length_b                   11.606
_cell_length_c                   11.702
_cell_volume                     1576.250
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Arakcheeva_KRISAJ_1995_1526.cif
_cod_data_source_block           Al0.11Ba2Cu2.725O6.4Tb0.182Y0.8
_cod_original_cell_volume        1576.25
_cod_database_code               1534631
The lanthanoid polyantimonides with the ideal compositions Pr5 Sb12 and Nd5 Sb12 crystallizing with a new structure type and Ho2 Sb5 with (Dy2 Sb5)-type structure
Schmidt, T.; Altmeyer, R.O.; Jeitschko, W.; Journal of Solid State Chemistry 173 (2003) 259–272; doi:

data_1534632
_publ_section_title
;
 The lanthanoid polyantimonides with the ideal compositions Pr5 Sb12 and
 Nd5 Sb12 crystallizing with a new structure type and Ho2 Sb5 with (Dy2
 Sb5)-type structure
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              259
_journal_page_last               272
_journal_volume                  173
_journal_year                    2003
_chemical_formula_sum            'Pr8.303 Sb20.03'
_space_group_IT_number           8
_symmetry_space_group_name_Hall  'C -2y'
_symmetry_space_group_name_H-M   'C 1 m 1'
_cell_angle_alpha                90
_cell_angle_beta                 95.52
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   28.591
_cell_length_b                   4.263
_cell_length_c                   13.561
_cell_volume                     1645.196
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Schmidt_JSSCBI_2003_763.cif
_cod_data_source_block           Pr8.303Sb20.03
_cod_database_code               1534632
Hg2 (O H) (B F4), the first basic mercurous tetrafluoroborate
Goebbels, D.; Meyer, G.; Zeitschrift fuer Anorganische und Allgemeine Chemie 629 (2003) 933–935; doi:

data_1534633
_publ_section_title
;
 Hg2 (O H) (B F4), the first basic mercurous tetrafluoroborate
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              933
_journal_page_last               935
_journal_volume                  629
_journal_year                    2003
_chemical_formula_sum            'B F4 H Hg2 O'
_chemical_name_systematic        'Hg2 (O H) (B F4)'
_space_group_IT_number           61
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   9.8504
_cell_length_b                   9.9096
_cell_length_c                   11.41
_cell_volume                     1113.770
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Goebbels_ZAACAB_2003_951.cif
_cod_data_source_block           H1B1F4Hg2O1
_cod_original_cell_volume        1113.77
_cod_original_formula_sum        'H1 B1 F4 Hg2 O1'
_cod_database_code               1534633